Fabrication, Characterization, and Energetic Properties of Metallized Fibers Nicholas A. Clayton,† Keerti S. Kappagantula,‡ Michelle L. Pantoya,‡ Sharon C. Kettwich,*,† and Scott T. Iacono*,† †
Department of Chemistry and Chemistry Research Center, United States Air Force Academy, 2355 Fairchild Drive, Suite 2N225, USAF Academy, Colorado 80840, United States ‡ Department of Mechanical Engineering, Texas Tech University, Lubbock, Texas 79409, United States ABSTRACT: Polystyrene ﬁbers loaded with an energetic blend of nanoaluminum (n-Al) and perﬂuoropolyether (PFPE) were successfully fabricated via electrospinning producing nanothermite fabrics. Fibers were generated with loadings up to 17 wt % n-Al/PFPE incorporated into the ﬁber. Microscopy analysis by SEM and TEM conﬁrm a uniform dispersion of PFPE treated n-Al on the outside and inside of the ﬁbers. Metallized ﬁbers were thermally active upon immediate ignition from a controlled ﬂame source. Thermal analysis by diﬀerential scanning calorimetry (DSC) found no change in glass transition temperature when comparing pure polystyrene ﬁbers with ﬁbers loaded up to 17 wt % n-Al/PFPE. Thermal gravimetric analysis (TGA) revealed a shift in decomposition temperatures to lower onsets upon increased loadings of n-Al/PFPE blends, consistent with previous studies. Flame propagation studies conﬁrmed that the metallized ﬁbers are pryolants. These metallized ﬁbers are a recent development in metastable intermolecular composites (MICs) and details of their synthesis, characterization, and thermal properties are presented. KEYWORDS: nanothermite, pyrolant, energetic material, electrospinning, nanoparticles
challenges associated with melt casting or ball milling of nanometallized propellants, for example, pre- or post-burning aggregation, can be mitigated. The technique of electrospinning has been around since the 1930s, but the mechanism behind the spinning was vaguely understood until the 1990s.17 For the most part, electrospinning is simple and versatile whereby ultrathin polymer composite and ceramic-based ﬁbers can easily be produced. In general, the morphology and diameter of electrospun ﬁbers are dependent on the intrinsic physical properties of the precursor solution (concentration, viscosity, and electrical conductivity) and the operating conditions (strength of the applied electric ﬁeld, distance between spinneret and substrate, and ﬂow rate of precursor solution).17 We have recently reported the fabrication of metallized energetic epoxide-based composites.15 An energetic blend of nanoaluminum (n-Al) coated with perﬂuoropolyether (PFPE) (Figure 1) was successfully loaded into a partially cured epoxide and allowed to fully cure. The resulting rigid material did not degrease beyond its glass transition temperature, is indeﬁnitely shelf-stable, and can be post-machined (drilled, milled, or Special Issue: Applications of Hierarchical Polymer Materials from Nano to Macro Received: October 17, 2013 Accepted: December 17, 2013 Published: December 31, 2013 6049
values.25 Initially, our attempts failed to eﬀectively electrospin Teﬂon AF dissolved in a variety of ﬂuorinated solvents (hexaﬂuorobenzene, Asahiklin AK-225, 3M Fluorinert FC75). It has been demonstrated that room temperature ionic liquids such as 1-butyl-3-methylimidazolium hexaﬂuorophosphate (BMIM-PF6) can be added to the precursor suspension with a similar partially ﬂuorinated, amorphous polymer in low amounts (>1.5 wt %) to make the suspension more electrospinnable.26 BMIM-PF6 was added to a suspension of Teﬂon AF® yet generation of ﬁbers via electrospinning was still unsuccessful. Teﬂon AF® has successfully been electrospun by implementing a coaxial electrospinning technique where an electrospinnable polymer is used as a so called guiding material to facilitate spinning.25,27,28 In one case, poly(vinylidene ﬂuoride) (PVDF) was used as a guiding material, but only 1 wt % Teﬂon AF® was successfully incorporated into ﬁbers.25 Instead of attempting coaxial electrospinning, polystyrene (PS) was chosen as the precursor polymer to be electrospun into ﬁbers. Lacking ﬂuorocarbon substitution, PS has a higher dielectric constant and has been employed in the commercial manufacture of electrospun ﬁbers; it was determined PS could serve as a suitable matrix material for this model study. We also attempted to electrospin ﬁbers loaded with n-Al only (no PFPE), but the metal particles would not remain as a stable suspension in PS/DMF. Similarly, when n-Al and PFPE were added to the PS/DMF solution independently (i.e., were not pre-coated), the constituents of the suspension would also separate. Polystyrene ﬁbers loaded with a uniform distribution of PFPE coated n-Al ﬁbers can only be produced when the precoating method is followed to prevent aggregation/agglomeration of the particles. The results are pictorially summarized in Figure 1; suspension separation was observed by eye; however, when photographed, the pictures failed to produce evident contrast. By not pre-coating the n-Al with PFPE, this causes separation of the suspension, clogging the syringe needle, and ultimately resulting in the inability to electrospin uniform metallized ﬁbers. The requirement of pre-coating the n-Al with the PFPE to make the particles miscible with the matrix was also observed when n-Al/PFPE blends were incorporated into epoxide matrices.15 Fiber diameters were determined via SEM and representative diameters for a range of ﬁber loadings are listed in Table 1 and SEM images are shown in Figure 2. As expected, the pure PS ﬁbers appear to have a smooth and regular surface morphology. Pure PS nanometer-sized ﬁbers were consistently achieved; however, upon loading with n-Al/PFPE, microﬁbers up to 5400 nm diameter were repeatedly achieved with no apparent correlation with wt% loading. A larger variation in diameter was observed for the 17 wt % n-Al/PFPE formulated ﬁbers (1900− 7900 nm) whereas electrospinning pure PS consistently produced ﬁbers <100 nm. The relatively wide range of ﬁber
Figure 1. TOP: Blending n-Al with PFPE-produced coated n-Al particles. BOTTOM: (a) When n-Al pre-coated with PFPE is added to a solution of PS/DMF, a viable suspension is formed and metallized ﬁbers can be electrospun. (b) If uncoated n-Al particles (no PFPE) are added to a solution of PS/DMF, the metal particles aggregate and settle out of solution so metallized ﬁbers cannot be electrospun. (c) If PFPE and n-Al are added separately to the PS/DMF solution, separation still occurs and metallized ﬁbers cannot be electrospun.
buﬀed) into any desirable shape without igniting the component metal, in this case, nanometer-sized aluminum. The metallized epoxide composite exothermically decomposes into the predominating metal-mediated oxidized AlF3 species as well as competing Al2O3 and Al4C3 as deﬂagration products. Based oﬀ of these initial ﬁndings, we were interested in studying if ﬁbers loaded with the energetic n-Al/PFPE blend could be electrospun in order optimize surface area between the fuel−oxidizer/core−shell particles and the matrix ﬁber dimensions.
RESULTS AND DISCUSSION When ﬁrst approaching the idea of electrospinning ﬁbers and loading them with an energetic blend of n-Al and PFPE, Teﬂon AF was chosen as the likely precursor polymer to enable electrospinning of the suspension in order to maximize ﬂuorine content of the bulk composite system. Pantoya et al. showed that reaction of micrometer- and nanometer-sized aluminum blended with polytetraﬂuoroethylene (PTFE or Teﬂon) is driven to proceed by extraction of ﬂuorine from the PTFE and formation of the thermodynamically stable species AlF3.18−20 This reaction is exothermic in nature and the reaction kinetics are well understood and extensively documented in the literature by numerous groups.1,21−24 Teﬂon AF, a copolymer of Teﬂon, seemed like a logical choice for ﬁber fabrication because it is a solution processable, amorphous thermoplastic. However, in practice, Teﬂon and Teﬂon AF are not conducive to electrospinning because of their low dielectric constant Table 1. Summary of Physical and Thermal Properties of Fibers entry PS standard PS ﬁbers n-Al/PFPE PS 1 n-Al/PFPE PS 2 n-Al/PFPE PS 3
calcd wt% Al/PFPE
exp wt% Al/PFPE
Al balc (%)
avg ﬁber ODa (SEM/nm)
ﬂame propag velocity (mm/s)
± ± ± ±
373 376 375 366 369
102 103 100 102 103
1.89 ± 0.07 1.94 ± 0.30 2.17 ± 0.80
5 10 15
6 10 17
1 1e 7 11 18
80 3900 1100 5400
20 400 400 2000
a Average of three electrospinning runs. bTGA onset of decomposition (5 °C/min) in nitrogen. cResidual n-Al balance recorded after 500 °C using TGA (5 °C/min) in nitrogen. dDSC (5 °C/min) in nitrogen determined by third heating cycle. eChar yield.
Figure 2. Electrospun control polystyrene ﬁbers (white) and PS ﬁbers loaded with 11 wt % n-Al/PFPE (dark grey) (top left). SEM images of: pure PS ﬁbers (top right), and PS ﬁbers electrospun with 6 wt % nAl/PFPE (lower left). TEM image of PS ﬁbers electrospun with 17 wt % n-Al/PFPE (lower right).
diameters suggests that while stock solutions appear as homogeneous suspensions, there is inhomogeneity with PFPE treated n-Al, leading to a size distribution of agglomerates. Figure 2 shows a SEM image of PS ﬁbers loaded with 6 wt % nAl/PFPE that have smooth surfaces and a varying range of diameters (3100−4300 nm). Interestingly, ﬁbers with 10 wt % n-Al/PFPE loadings produced consistently the smallest size distribution (700−1500 nm). TEM analysis showed that the nAl agglomerates are uniformly distributed on the surface of the ﬁbers. A representative TEM image is shown in Figure 2 with a loading of 17 wt % n-Al/PFPE. The particles appear to be evenly distributed as aggregated of 200−500 nm along the edges of the ﬁber and are also embedded in the core of the ﬁber. PS ﬁbers with loadings higher than 17 wt % n-Al/PFPE could not be generated. Varying experimental parameters (viscosity of suspension, working voltage, ﬂow rate, substrate distance, needle gauge) still failed to produce uniform ﬁbers, but rather formed an agglomerated material at higher concentrations. Yan et al. observed similar agglomeration when electrospinning nitrocellulose based ﬁbers and trying to maximize the mass loading of Al/CuO to make energetic thermite textiles.16 They found that at loadings above 50 wt % nanothermite, the Taylor cone became increasingly unstable, thereby causing severe particle agglomeration. The thermal stability of the composite ﬁber system was studied employing TGA and DSC; the resulting measurements for representative ﬁbers are summarized in Table 1. TGA plots of standard PS compared to PS ﬁbers and ﬁbers loaded with nAl/PFPE blends are shown in Figure 3. Onset of decomposition (Td) of PS ﬁbers occurs at 376 °C, which agrees with the observed decomposition of standard PS at 373 °C. Low loadings of 6 wt % up to 17 wt % n-Al/PFPE blends did not appear to aﬀect the decomposition temperatures of the ﬁbers. PS and PFPEs are well known to decompose at temperatures >350 °C into volatile aromatic compounds producing char yields <1%.29−31 For samples loaded with n-Al/PFPE, remaining mass balances are equivalent to the amount of nAl loaded in the ﬁbers. As seen in Figure 3, at temperatures above the melting transition of Al (Tm of 660 °C), the metal begins to oxidize and the mass balance increases.32 DSC
Figure 3. TOP: TGA in N2 of the standard PS (blue), electrospun PS ﬁbers (red), ﬁbers loaded with 6 wt % n-Al/PFPE blend (black), and ﬁbers loaded with 17 wt % n-Al/PFPE blend (green). BOTTOM: DSC plots of PS ﬁbers (red), ﬁbers loaded with 6 wt % n-Al/PFPE blend (black), and ﬁbers loaded with 17 wt % n-Al/PFPE blend (green). Y-axis plotted as exotherm up and plots have been normalized to zero at Tg.
analysis was performed on all samples and selected plots are also shown in Figure 3. The glass transition temperature (Tg) did not change upon addition of n-Al/PFPE blend (Tg of 102 °C) which is consistent with previous studies on metallized PFPE epoxides. Unlike previous studies, the enthalpy (ΔH) of the thermally-induced Al−F formation could not be determined via DSC. Plots are normalized with respect to Tg, yet a discrete exothermic event could not be distinguished even when comparing pure PS ﬁbers with ﬁbers loaded with the fueloxidizer blend. The presence of aluminum in the highest loadings (17 wt % n-Al/PFPE) serves to slightly catalyze degradation of the ﬁbers to an onset of 369 °C; this highest nAl-loaded composite system still appears to be a suitable for repetitive high temperature service conditions. Because thermal analysis did not provide insight into the exothermic nature of the degradation of the samples, ﬂame propagation velocities of composite ﬁbers were determined in addition to thermal analysis. Flame propagation velocities of diﬀerent samples with varying weight percent loadings of n-Al/ PFPE (6−17 wt % n-Al/PFPE) were determined. A schematic of the experimental set-up employed for the determination of the ﬂame propagation velocity of the aluminum-ﬂuoropolymer 6051
ﬁber composite is shown in Figure 4. Rectangular strips of the ﬁbers with 100 mm length and 10 mm width were cut and
Precursor Solution. To prepare the PS solution, 30 wt % bulk PS pellets (commercially available, Mn of 270 000 g/mol by GPC) were dissolved in N,N-dimethylformamide (DMF, anhydrous, 99.8%, Acros Organics) overnight, at 50 °C in a heater/shaker. Before incorporation into the PS carrier solution, 30 wt % n-Al (US Army Armament Research, Development, and Engineering Center-ARDEC, ca. 80 nm (by TEM), 70% active, ca. 2−5 nm oxide shell) was blended with PFPE (Sigma-Aldrich, Fomblin® Y LVAC 25/6, 3300 g/mol) in a glove box (MBraun Labmaster) under nitrogen. Blends of n-Al/PFPE are weighed directly into a glass screw cap vial and are typically prepared on the 1 g scale. Blends are manually mixed with a spatula for 5 min, capped, and ﬁnally removed from the glove box for ﬁber preparation. Previous experimental studies employing PFPEs to coat diﬀerent weight percent n-Al revealed the optimized stoichiometric ratio producing the largest enthalpy of reaction (ΔH) to be 30 wt % n-Al fuel to 70 wt % PFPE oxidizer.15 Thus, a blend of 30 wt % n-Al in PFPE is implemented in the current study to prepare ﬁbers. The desired amount of n-Al/PFPE blend is added to the PS/DMF solution. The suspension is manually mixed with a spatula for 5 min and then ultrasonicated for 5 mins. The suspension is immediately electrospun within 10 min. If the suspension is not immediately used for ﬁber preparation, the solids irreversibly precipitate out of the DMF solution as a solid block within 12 h. Weight percent loadings of n-Al were initially calculated and weighed in order to prepare the precursor solution. After ﬁbers were electrospun, the sample was measured to determine the residual Al content at 500 °C using TGA (5 °C/min) in nitrogen which was used to back-calculate the n-Al/PFPE loading. These measurements were performed because although the precursor suspensions are relatively stable for short periods of time (<0.5 h), some settling out of the Al does occur altering the transferred mass balance during electro-spinning. Fiber Spinning. An in-house electrospinning setup in a fume hood is used to electrospin the metallized suspension equipped with syringe pump (KD Scientiﬁc model 100 syringe pump), target plate, and accompanying voltage supply (EL Glassman High Voltage source). In order to reduce the chance of spark ignition while electrospinning, a low working voltage of 12−15 kV, is applied to a stainless steel needle (17−27 gauge) thereby charging the n-Al/PFPE loaded PS/DMF suspension. The syringe pump is set at a ﬂow rate of 0.5−1.25 mL/h and non-woven ﬁber mats are collected 76−100 mm from the needle tip onto a square target plate (75 mm × 75 mm) covered in aluminum foil. Control PS ﬁbers without any n-Al or PFPE were also electrospun using the conditions discussed above in order to validate the reproducibility of the electrospinning apparatus. When loaded with a blend of PFPE coated n-Al particles, the ﬁbers become dark grey and appear denser than the control PS ﬁbers without any additives (Figure 2). Thermal Analysis and Microscopy Characterization. Thermal gravimetric analysis (TGA) and diﬀerential scanning calorimetry (DSC) was performed on a TA Q500 and TA Q20, respectively. Measurements were performed under N2 atmosphere at a rate of 5 °C/min. Scanning electron microscopy (SEM) and transmission electron microscopy (TEM) was performed on a Hitachi S-4800 (Clemson University Electron Microscopy Facility) or a JEOL 6460 LV and Hitachi H-7600 (Clemson University Electron Microscopy Facility), respectively. Flame Propagation Analysis. A Phantom v7 (Vision Research, Inc., Wayne, NJ) with a Nikon AF Nikkor 52 mm 1:2.8 lens was used to record ignition and ﬂame propagation of the mixtures. The camera captured images of the burning ﬁber composite, perpendicular to the direction of ﬂame propagation, with a resolution of 256 × 128 pixels.
Figure 4. LEFT: Schematic for ﬂame propagation experiments. RIGHT: High speed video camera footage displaying sequential snapshots of 17 wt % n-Al/PFPE ﬁbers burning. Fibers are ignited on the right and the ﬂame front propagates to the left.
rolled to obtain a cylindrical cross section along the length of the ﬁber. These samples were then placed inside a steel combustion chamber (48 × 48 × 48 mm) at room temperature and pressure and ignited using a match. Figure 4 shows sequential snapshots of the progression of the ﬂame front of the ﬁbers burning in the air. Graphical software was used to post-process the recorded photographic data. With an established reference, the software determined ﬂame velocity based on a distance between sequential time frames. Using a “ﬁnd edge” image ﬁlter that identiﬁed preset variations in pixel intensity, the ﬂame front location (which was assumed as the region of the ﬂame with the maximum radiance) was identiﬁed and marked for velocity measurements. Three tests were conducted on each sample to ensure repeatability of ﬂame propagation velocity measurements and a summary of the results are shown in Table 1. Polystyrene ﬁbers loaded with low amounts of n-Al/PFPE (6 wt %) were found to have a combustion velocity of 1.89 ± 0.30 mm/s and increasing the n-Al/PFPE loading to 17 wt % increased the ﬂame propagation velocity to 2.17 ± 0.80 mm/s. On the basis of the determined ﬂame propagation velocities, the loaded ﬁber composites are slow burning pyrolants reacting at subsonic speeds <1 m/s and higher n-Al loadings do not appear to inﬂuence the rates given the standard deviation in velocities. As a comparison with the only recent report of electrospun pyrolant-based ﬁbers, electrospun nitrocellulose ﬁbers loaded with 50 wt % n-Al/CuO produced reactive textiles that were also found to react at subsonic speeds, albeit about three orders of magnitude faster than n-Al/PFPE ﬁbers at ca. 100 cm/s.16 This separation implies usefulness for very diﬀerent applications where propulsion versus localized energy generation as in the case for micro-electro-mechanical systems (MEMS), for example, may be required.
CONCLUSION In summary, we were able to successfully electrospin polystyrene ﬁbers loaded with an energetic formulation of nAl particles pre-coated with PFPE. Thermal analysis revealed that increased loadings of n-Al/PFPE results in a decrease in 6052
(16) Yan, S.; Jian, G.; Zachariah, M. R. ACS Appl. Mater. Interfaces 2012, 4, 6432. (17) Li, D.; Xia, Y. Adv. Mater. 2004, 16, 1151. (18) Watson, K. W.; Pantoya, M. L.; Levitas, V. I. Combust. Flame 2008, 155, 619. (19) Hunt, E. M.; Malcolm, S.; Pantoya, M. L.; Davis, F. Int. J. Impact Eng. 2009, 36, 842. (20) Dikici, B.; Dean, S. W.; Pantoya, M. L.; Levitas, V. I.; Jouet, R. J. Energ. Fuel. 2009, 23, 4231. (21) Koch, E.-C. Propell. Explos. Pyrotech. 2002, 27, 340. (22) Koch, E.-C. In Handbook of Combustion; Lackner, M., Winter, F., Agarwal, A. K., Eds.; Wiley: Weinheim, Germany, 2010; Vol. 5, p 355. (23) Pantoya, M. L.; Dean, S. W. Thermochim. Acta 2009, 493, 109. (24) Dolgovorodov, A. Y.; Makhov, M. N.; Kolbaney, I. V.; Streletskii, A. N.; Fortov, V. E. JETP Lett. 2005, 81, 311. (25) Muthiah, P.; Hsu, S.-H.; Sigmund, W. Langmuir 2010, 26, 12483. (26) Verma, R.; Tomar, N.; Creager, S. E.; Smith, D. W., Jr. Polymer 2012, 54, 2211. (27) Greiner, A.; Wendorff, J. H. Angew. Chem. 2007, 46, 5670. (28) Maghe, A. K.; Gupta, B. S. Polym. Rev. 2008, 48. (29) Onwudili, J. A.; Nagi, I.; Williams, P. T. J. Anal. Appl. Pyrol. 2009, 86, 293. (30) Filip, M. R. P.; Aurelia; Rusu, T. Studia UBB Chemia 2011, 56, 27. (31) Scheirs, J. In Modern Fluoropolymers; Scheirs, J., Ed.; Wiley: New York, 1997, p 637. (32) CRC Handbook of Chemistry and Physics, 84th ed.; CRC Press: Boca Raton, FL, 2003.
temperatures of decomposition consistent with previous work on epoxy-based metallized bulk composites. Flame propagation studies conﬁrm similar combustion rates with increased loadings of the energetic blend into the ﬁbers. Electrospinning of energetic ﬁbers is a novel way to prepare pyrolant mats. Selecting other polymer systems to electrospin with n-Al/PFPE blends in order to explore other morphologies may increase the ﬂame propagation velocities of ﬁbers, and would be the next logical concentration for on-going work.
The manuscript was written through contributions of all authors. All authors have given approval to the ﬁnal version of the manuscript. Notes
The authors declare no competing ﬁnancial interest.
ACKNOWLEDGMENTS The authors acknowledge Dr. Laxmikant Saraf and George Wetzel (Clemson University Electron Microscopy Facility) for the SEM and TEM images and Ryan Steelman (Texas Tech University) for technical expertise. S.C.K. acknowledges funding for this work made available by Air Force Research Laboratory, Eglin Air Force Base, sponsored by the U.S. Air Force Academy under Agreement FA7000-10-2-0038. M.L.P. acknowledges support from the US Army Research Oﬃce Contract W911NF1110439.
(1) Koch, E.-C. Metal-Fluorocarbon Based Energetic Materials; Wiley: Weinheim, Germany, 2012. (2) Crouse, C. A.; Pierce, C. J.; Spowart, J. E. Combust. Flame 2012, 159, 3199. (3) Kappagantula, K.; Pantoya, M. L.; Hunt, E. M. J. Appl. Phys. 2012, 112, 1. (4) Sippel, T. R.; Son, S. F.; Groven, L. J. Propell. Explos. Pyrotech. 2013, 38, 286. (5) Manukyan, K. V.; Mason, B. A.; Groven, L. J.; Lin, Y.-C.; Cherukara, M.; Son, S. F.; S Strachan, A.; Mukasyan, A. S. J. Phys. Chem. C 2012, 116, 21027. (6) Kim, S. H.; Zachariah, M. R. Adv. Mater. 2004, 16, 1821. (7) Kappagantula, K. S.; Farley, C.; Pantoya, M. L.; Horn, J. J. Phys. Chem. C 2012, 116, 24469. (8) Wu, C.; Sullivan, K.; Chowdhury, S.; Jian, G.; Zhou, L.; Zachariah, M. R. Adv. Funct. Mater. 2012, 22, 78. (9) Yetter, R. A.; Risha, G. A.; Son, S. F. Proc. Comb. Inst. 2009, 32, 1819. (10) Koch, E.-C.; Metal-Fluorocarbon Based Energetic Materials; Wiley: Germany, 2012, pp 42−67. (11) Slocik, J. M.; Crouse, C. A.; Spowart, J. E.; Naik, R. R. Nano Lett. 2013, 13, 2535. (12) Crouse, C. A.; Pierce, C. J.; Spowart, J. E. ACS Appl. Mater. Interfaces 2010, 2, 2560. (13) Christopher, A. C. In Advances in Fluorine-Containing Polymers; American Chemical Society: Washington, D.C., 2012; Vol. 1106, p 127. (14) Martin, M.; Hanagud, S.; Thadhani, N. N. Mater. Sci. Eng. A 2007, 443, 209. (15) Miller, H. A. K.; Bradley, S.; Danielson, S. T.; Neat, J. W.; Avjian, E. K.; Pierson, S. N.; Budy, S. M.; Ball, D. W.; Iacono, S. T.; Kettwich, S. C. J. Mater. Chem. A 2013, 1, 7050. 6053
A major goal of biomimetics is the development of chemical compositions and structures that simulate the extracellular matrix. In this study, gelatin-based electrospun composite fibrous membranes were prepared by electrospinning to generate bone scaf
Herein, novel hybrid nanomaterials were developed for wound dressing applications with antimicrobial properties. Electrospinning was used to fabricate a double layer nanocomposite nanofibrous mat consisting of an upper layer of poly(vinyl alcohol) an
Micro- and nanomechanical string resonators, which essentially are highly stressed bridges, are of particular interest for micro- and nanomechanical sensing because they exhibit resonant behavior with exceptionally high quality factors. Here, we fabr
The objective of this study was to fabricate and characterize electrospun fibers loaded with budesonide with the aim of controlling its release in the gastrointestinal tract. Budesonide is a nonhalogenated glucocorticosteroid drug, highly effective i
Inspired by the high adhesiveness of the electrospun fiber, we propose a method to fabricate multi-scale heterogeneous hump-on-string fiber via the adsorption of nanoparticles, the NPCTi which is the hydrolysate of titanium tetrachloride (TiCl₄) and
This study demonstrates the fabrication of κ-carrageenan fibers by a wet-spinning method and discusses three important spinning parameters: coagulation bath composition, spinning rate and post-spinning mechanical drawing. The as-spun fiber diameter d
Here we report a one-pot route for the synthesis of nickel dodecahedra with 52.3 ± 0.1 emu g(-1) of saturation magnetization. The procedure is very simple, and only three chemicals (NiCl2·6H2O, isopropanol and polyvinylpyrrolidone) are used throughou
In this study, TiO2 nanotubes were fabricated using anodic oxidation in fluoride containing weak organic acid for different durations (0.5h, 1h, 2h and 3h). Scanning electron microscope (SEM) micrographs reveal that the morphology of titanium oxide v
Ankyrin repeat containing proteins are one of the most abundant solenoid folds. Usually implicated in specific protein-protein interactions, these proteins are readily amenable for design, with promising biotechnological and biomedical applications.
Using a variety of functionalization strategies, derivatives of 4, 4'-bis(5-nitro-1,2,3-2H-triazole) were designed, synthesized, and characterized. The isomers were separated, their structures were confirmed with single-crystal X-ray analysis, and th